Determination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors


 Amelia Johns
 1 years ago
 Views:
Transcription
1 Sensors 2012, 12, ; doi: /s Article OPEN ACCESS sensors ISSN Determination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors Jin Y. Park 1 and Jeong Wan Lee 2, * 1 2 Mechanical Engineering, Minnesota State University, Mankato, MN 56001, USA; Mechanical and Mechatronics Engineering, Kangwon National University, 1 Kangwondaehakgil, Chuncheonsi, Gangwondo , Korea * Author to whom correspondence should be addressed; Tel.: ; Fax: Received: 27 August 2012; in revised form: 5 November 2012 / Accepted: 5 November 2012 / Published: 22 November 2012 Abstract: This paper presents a method and procedure of sensing and determining critical shear buckling load and corresponding deformations of a comparably large composite Isection using strain rosettes and displacement sensors. The tested specimen was a pultruded composite beam made of vinyl ester resin, Eglass and carbon fibers. Various coupon tests were performed before the shear buckling test to obtain fundamental material properties of the Isection. In order to sensitively detect shear buckling of the tested Isection, twenty strain rosettes and eight displacement sensors were applied and attached on the web and flange surfaces. An asymmetric fourpoint bending loading scheme was utilized for the test. The loading scheme resulted a high shear and almost zero moment condition at the center of the web panel. The web shear buckling load was determined after analyzing the obtained test data from strain rosettes and displacement sensors. Finite element analysis was also performed to verify the experimental results and to support the discussed experimental approach. Keywords: strain sensor; displacement sensor; shear buckling; polymer composite Isection; asymmetric loading
2 Sensors 2012, Introduction An Isection beam consists of two panels of flanges and a web panel. When loaded, the Isections are subjected to combined axial (or normal) and shear stress fields. It is wellknown that the web panel does most of work in resisting the shear force [1,2]. The shear force often causes a critical condition of failure of a loaded Isection. For instance, inclined cracks or damage patterns are easily observed from tested metal Isections. The inclined cracks or patterns in a deep beam show the existence of shear in the web. If a web height is large enough (a deep beam with span/depth < 6), member capacity is usually governed by the shear behavior of the web material. Since the early 1990s, many researchers have studied the buckling of fiber reinforced polymer (FRP) composite members: Barbero and Raftoyiannis reported analytical and experimental approaches to buckling of pultruded FRP columns [1,2]. Motram [3] published his study on pultruded composites lateraltorsional buckling for the first time. Bank [4] and his colleagues published a paper describing their effective lateral buckling test method for composite beams. In 2002, Roberts [5] published that a shear deformation could significantly influence the buckling behavior of a composite Isection under any loading scheme. Shan and Qiao [6] proposed a test method and theoretical verification using energy theory for flexural torsional buckling of an open channel beam. Many other recent papers [7 11] have described theoretical and experimental approaches to buckling of composite members and concluded by mentioning the important effect of shear behavior on buckling. However, a full experimental approach to obtain the shear buckling load of large polymer composite Isections has not been studied much yet. This is because a pure shear stress state is very difficult to achieve experimentally with a large span composite Isection. In this study, a test method to detect and determine the critical shear buckling load and to observe the buckling behaviors of a comparably large pultruded composite Isection was discussed. An asymmetric shear loading scheme was proposed and utilized for the test program. In order to sensitively obtain the shear buckling load and shear behavior of the composite Isection, twenty strain rosette sensors were attached on the web surface of the Isection. The tested section was also instrumented at various locations with displacement sensors to indicate lateral and vertical displacements of the web. Finite Element Analysis (FEA) was also performed. The results from the FEA were compared with those from the experimental test to verify and support the discussed experimental method. 2. Experimental Section 2.1. The Tested ISection The tested composite girder was a 4,572 mm long Ishaped section having the crosssectional dimensions shown in Figure 1(a). The web was reinforced with a total of six layers: these are two layers of Eglass rovings and three layers of randomly oriented Eglass Continuous Strand Mat (CSM) not 6. The top and bottom flanges were reinforced with eleven Eglass/carbon hybrid rovings combined with Eglass CSM layers for each; four layers of carbon roving, a layer of Eglass roving and six layers of Eglass CSM. The reinforcing scheme for the web and flanges are shown in Figure 1(b).
3 Sensors 2012, Figure 1. The crosssectional dimensions and reinforcing scheme of the test component. (a) Cross sectional dimension; (b) Reinforcing scheme. (a) (b) The weight fractions of the composite constituents of the web were examined following the technique described in Ye et al. [12], which was based on ASTM D 2584 [13]. Regarding the weight fractions of the constituents of the flanges, the technique described in ASTM D 3171 [14] was used. Since the carbon fibers are oxidized during a burnout process, the technique outlined in Ye et al. [12] could not be utilized for the flange elements. Thus, digestion in nitric acid 70% solution was performed. After digestion for 168 h (1 week), the carbon and glass fibers were rinsed with acetone and water. The average weight and computed volume fractions of all constituents of the web and the flange elements are listed in Table 1. Table 1. Average weight and volume fractions of the constituents (four samples each). Location Constituents Weight Fraction (%) STD * (%) COV ** (%) Volume Fraction (%) Web Vinylester resin Eglass roving Eglass CSM Clay fillers Voids Flange Vinylester resin Eglass roving Carbon roving Eglass CSM Clay fillers Voids * STD: Standard deviation; ** COV: Coefficient of variation. STD (%) CO (%)
4 Sensors 2012, Material Properties Figure 2 shows both the member s global coordinate system (X, Y, Z) and the member elements local coordinate system (x, y and z). The tensile, compressive and shear properties of the web materials of the pultruded composite Ishaped section specimen were determined according to ASTM D 3039 [15], ASTM D 3410 [16] and ASTM D 5379 [17], respectively. Figure 2. Global and local coordinate system. The mechanical properties of the flange material of the specimen were also determined. Since the flanges do not have symmetric layups, a flexural coupon test [18,19] was also carried out to obtain the extensional properties of the flange. For this flexural coupon test, twenty samples were cut from the top and bottom flanges in the xdirection. The obtained mechanical properties of the flange material are tabulated in Table 2. Table 2. Mechanical property values of the flanges. Test Loading direction Constants Average COV (%) Flexural Shear Group I * (10 samples) Group II ** (10 samples) xyshear direction (10 samples) E b x 25.8 GPa 7.1 σ ub x 347 MPa 5.5 ε ub x 1.50% 11.5 E b x 27.3 GPa 7.1 σ ub x 436 MPa 5.3 ε ub x 1.48% 16.2 G xy 3.8 GPa 6.4 τ u xy 99.5 MPa 3.4 γ u xy 4.14% 10.2 * Group I ** Group II
5 Sensors 2012, , and in the table are flexural modulus, flexural ultimate strength and strain of the flange in the xdirection, respectively. The test results from the flexural tests can be divided into two groups (Group I and Group II) according to the layup sequence shown in Table 2. The material properties of the web material are summarized in Table 3.,, and in the table are extensional modulus, ultimate strength, ultimate strain and Poison s ratio of the web in the xdirection, respectively.,, and in the table are extensional modulus, ultimate strength, ultimate strain and Poison s ratio of the web in the ydirection, respectively. The superscript t indicates tensile loading direction. The compressive modulus, compressive ultimate strength, compressive ultimate strain and Poison s ratio of the web are also listed in Table 3. The superscript c indicates compressive loading direction. Shear modulus (G xy ), strength ( ) and strain ( ) are also shown in Table Experimental Setup Table 3. Mechanical property values of the web. Test Loading direction Constants Average COV (%) E t x 18.9 GPa 6.9 xdirection σ ut x MPa 13.4 (10 samples) ε ut x Tensile ν t xy E t y 9.99 GPa 2.3 ydirection σ ut y 89.0 MPa 3.0 (10 samples) ε ut y ν t yx E c x 20.4 GPa 7.4 xdirection σ uc x MPa 9.8 (10 samples) ε uc x Compressive ν c xy E c y 11.5 GPa 6.7 ydirection σ uc y MPa 7.4 (10 samples) ε uc y ν c yx xyshear G xy 4.3 GPa 9.3 Shear direction τ u xy 96.9 MPa 6.2 (10 samples) γ u xy Figure 3 shows a sketch of the test component subjected to four point asymmetric loading. Due to the asymmetric loading pattern, there is the maximum vertical shear force applied at the center of the specimen. Bending moment should be theoretically zero at the center of the beam. At the support and load application points, transverse stiffeners on both sides of the web were provided. A total of eight Eglass/vinylester tubular sections having nominal dimensions of mm mm 9.53 mm were used as transverse stiffeners. The girder was restrained against lateral movement by means of a total of eight steel plates having dimensions of 76.2 mm 381 mm 12.7 mm and the transverse stiffeners at the support and load application points. A spreader beam was placed between the load actuator and
6 Sensors 2012, two bearing plates to apply the asymmetric loading to the specimen. By this loading mechanism, the applied load P was divided into 0.73 P and 0.27 P at the shown bearing contacts. A photograph of the test setup is shown in Figure 4. Figure 3. Asymmetric loading test setup. Figure 4. A photograph of asymmetric four point loading setup Sensor Application The instrumentation in the girder consisted of strain rosettes manufactured by Vishay (CEA125UR350) and displacement sensors that were Celesco PT1A string potentiometers with up to 254 mm measurement capacity and accuracy of 0.15% of full stroke range. Twenty strain rosette sensors were used to measure 45, +45 and 0 directional strains as shown in Figure 5. Seventeen strain rosettes were attached on one side of the web and the other three strain rosettes were located on the other side of the web. The identifications of the strain rosettes are shown in Figure 6. Three locations (A4, B2 and C1) were selected for backtoback strain rosette applications to accurately determine the strains near buckling. Outofplane bending could also be observed by the measurement of the strains from the backtoback rosettes at these points. Seven strain rosettes were aligned vertically on the center line AA. Five strain rosettes were located on line BB mm from AA. Five strain rosettes are also located on line CC mm from AA. A photograph of the rosettes installed on the web surface is shown in Figure 7.
7 Sensors 2012, Figure 5. Locations of strain rosettes and displacement sensors on the bottom flange. Figure 6. The identification of strain rosettes on the web surface. A total of eight displacement sensors were used to measure the vertical and lateral deflections of the web. Seven locations, including two supporting points, were selected to measure vertical deflections using the potentiometers. They were V 1, V 2, V 3, V 4, V 5, V 6 and V 7 as shown in Figure 6. The vertical deflections at the supporting points (V 1 and V 5 ) were obviously zero. The locations of the potentiometers are also shown in Figure 7. Figure 8 shows the locations of three additional displacement sensors used to measure the lateral deflections (L 1, L 2 and L 3 ) of the web at the center of the Ishaped section.the load was applied to the top of the load spreader as shown in Figures 4 and 5. The applied load was continuously increased to the failure point at which the webflange junction fractured. An MTS 894 kn capacity load generator was used. The girder then was unloaded. The loading and unloading rates were 1.27 mm/s. The data were recorded electronically at a rate of 0.5 Hz.
8 Sensors 2012, Figure 7. A photograph of strain rosettes on the web. Figure 8. Locations of displacement sensors on the web surfaces. 3. Results and Discussion 3.1. Test Results Loadvertical deflection curves at five locations along the bottom of the lower flange are shown in Figure 9. The vertical deflections were measured using displacement sensors. Figure 9. Measured bottom flange vertical displacements.
9 Sensors 2012, Figure 10 shows the lateral web displacements measured by potentiometers at three locations of the center of the girder. Figure 10. Web outofplane displacements at section AA. Figures show the shear strains in the xy plane γ xy, the difference in the shear strain values obtained from the backtoback gages (γ xy ) 1 and (γ xy ) 2, and the average value of the shear strain γ xy at locations A4, B2 and C1, respectively. All Figures show clearly that prior to buckling the loadstrain behavior were close to linear. The values of γ xy were determined along with the axial strains from Equation (1) and the strain values recorded from the strain rosettes: where ε i s are direct strain sensor readings from three sensors in a rosette, and θ i s are the orientation of the three strain gages Determination of Shear Buckling Load 2 2 ε = ε cos θ + ε sin θ + γ cosθ sinθ ( i = 1,2,3) i x i y i The experimental buckling load was estimated from the loadlateral displacement curves obtained from the displacement sensors (Figure 10) and from the loadstrain relation curves determined by the data points of strain rosettes (Figures 11 13). It was determined by taking the intersection point of the tangent drawn to a curve before and after buckling as outlined by Hoff, et al. [20]. This method is a wellknown method called Bifurcation method. It is based on the phenomenon that the web surface should be sharply deformed at the moment of buckling. The critical load was determined by applying projection of the intersection onto the loaddisplacement and loadstrain curves. Any analytical equation was not used to determine a shear buckling load in this study. The evaluation results for the experimental buckling load by the data curves in Figures were very consistent. Table 4 lists the evaluated shear buckling loads from the four data sets. Since the values were close enough, arithmetic means were calculated and listed. The determined shear buckling load was 295 kn. xy i i (1)
10 Sensors 2012, Figure 11. Loadshear strain at location A4. (γxy) 1 (γxy) 2 (γxy) 1 [(γxy) 1 +(γxy ) 2 ]/2 (γxy) 2 Figure 12. Loadshear strain at location B2. (γxy) 2 (γxy) 1 (γxy) 1 (γxy) 2 [(γxy) 1 +(γxy) 2 ]/2 Figure 13. Loadshear strain at location C1. (γxy) 1 (γxy) 2 (γxy) 1 (γxy ) 2 [(γxy) 1 +(γxy) 2 ]/2
11 Sensors 2012, Table 4. The determined shear buckling loads (unit: kn). Lateral displacements Back to back Shear Strains at A4 Back to back Shear Strains at B2 Back to back Shear Strains at C1 Sensor positions W 1 W 2 W 3 (γ xy ) 1 (γ xy ) 2 (γ xy ) 1 (γ xy ) 2 (γ xy ) 1 (γ xy ) 2 Shear buckling load Finite Element Analysis The shear buckling load was also obtained using finite element computer program ABAQUS. The specimen was modeled three dimensionally using S8R5 element (8node doubly curved thick shell, reduced integration). Figure 14 shows the finite element model of the Ishaped section. The specimen was modeled using a total of 1,800 elements and 6,345 nodes, which resulted in relatively fine mesh of which element aspect ratios were 1.08 for the web and 1.07 for the flange. Figure 14. Finite element analysis; buckled shape of the deep composite Ishaped section. The orthotropic material properties determined using the coupon test results (Section 2.2) were used and the outofplane shear moduli (G zx and G yz ) were assumed to be the same as inplane shear modulus (G xy ). The loading and support points were identical to the experimental conditions. The bottom supports were modeled by restraining outofplane displacements and vertical movements. The node in the center of the bottom flange at a supported region was restrained against longitudinal translation to prevent a rigid body motion. The lateral (outofplane) displacements on the loading line were inhibited by the lateral supports and the loading areas on the top flange were also restrained in outofplane direction. The laterally supported areas on the web were also restrained in rotations and the displacement in the outofplane direction. The total load P was divided into two forces P 1 and P 2 that had magnitudes of 0.73 P and 0.27 P, respectively to simulate the actual experimental loading conditions. The loads P 1 and P 2 were applied to the top flange as pressures on the area of 152 mm 191 mm. This area was identical to that of the bearing plates placed on the top flange for the test. The stiffeners shown in Figure 4 were not included in the FEM modeling. Simplified displacement constraint conditions were applied instead: The lateral displacements of the web were assumed to be zero on the contact surfaces. The rotations about the longitudinal axis at the contacts were also fixed. Since the pure shear spot theoretically existed at the
12 Sensors 2012, center of the testsection, the effect to the shear buckling load due to the usage of the stiffeners was not considered significant. The shear buckling load was determined by taking the lowest positive eigenvalue (first mode of buckling). The critical buckling load obtained from the finite element analysis was 292 kn. Figure 14 shows the buckled shape of the Ishaped section. The displacement magnification factor in the figure is 7.0. Additional postprocessing figures with static and buckling analyses are also available [21]. 4. Conclusions In this study, the buckling of a pultruded polymer composite Ishaped section under shear loading was investigated experimentally. Based on the results, the following conclusions were derived: (1) The presented shear buckling test method using an asymmetric loading scheme effectively generated a shear loading condition and a pure shear region on the web of the tested Isection. (2) The corresponding displacements and shear strains were successfully obtained from the displacement and strain sensors, and they were used to observe the shear buckling behaviors of tested composite Isection. (3) In order to determine shear buckling load experimentally, a classical approach presented by Hoff, et al. was used. The results of shear buckling loads from loadlateral displacements relations, and loadshear strain at three different locations were very close. (4) The critical shear buckling load experimentally obtained was 295 kn. (5) In order to verify the experimental results, a finite element analysis was performed. The obtained shear buckling load was 292 kn. The analysis results support the validity of the presented experimental approach. Acknowledgments This study was supported by 2010 Research Grant from Kangwon National University, Korea. References 1. Barbero, E.J.; Raftoyiannis, I. Local buckling of FRP beams and columns. ASCE J. Mater. Civil Eng. 1993, 5, Barbero, E.J.; Raftoyiannis, I. Lateral and distortional buckling of pultruded Ibeams. Compos. Struct. 1994, 27, Mortram, J.T. Lateraltorsional buckling of a pultruded Ibeam. Composites 1992, 23, Bank, L.C.; Nadipelli, M.; Gentry, T.R. Local buckling and failure of pultruded fiberreinforced plastic beams. J. Appl. Mater. Technol. 1994, 116, Roberts, T.M. Influence of shear deformation on buckling of pultruded fiber reinforced plastic profiles. J. Compos. Construct. 2002, 6, Shan, L.; Qiao, P. Flexural torsional buckling of fiberreinforced plastic composite open channel beams. Compos. Struct. 2005, 68, Qiao, P.; Davalos, J.F.; Wang, J. Local buckling of composite FRP shapes by discrete plate analysis. J. Struct. Eng. 2001, 127,
13 Sensors 2012, Bazant, Z. Shear buckling of sandwich, fiber composite and lattice columns, bearings, and helical springs: Paradox resolved. J. Appl. Mech. 2003, 70, Karama, K.S.; Mistou, A.S. Mechanical behavior of laminated composite beam by the new multilayered laminated composite structures model with transverse shear stress continuity. Int. J. Solid. Struct. 2003, 40, Singer, J.; Arbocz, J.; Weller, T. Frontmatter. In Buckling Experiments: Experimental Methods in Buckling of ThinWalled Structures: Shells, BuiltUp Structures, Composites and Additional Topics; John Wiley & Sons, Inc.: Hoboken, NJ, USA, 2008; Volume 2, pp Xu, R.; Wu, Y. Static, dynamic and buckling analysis of partial interaction composite members using Timoshenko s beam theory. Int. J. Mech. Sci. 2007, 48, Ye, B.S.; Svenson, A.L.; Bank, L.C. Mass and volume fraction properties of pultruded glass fiberreinforced composites. Composites 1995, 26, American Society for Testing and Materials (ASTM). ASTM D 2584, Standard Test Method for Ignition Loss of Cured Reinforced Resins; ASTM: Englewood, CO, USA, American Society for Testing and Materials (ASTM). ASTM D 3171, Standard Test Methods for Constituent Content of Composite Materials; ASTM: Englewood, CO, USA, American Society for Testing and Materials (ASTM). ASTM D 3039, Standard Test Method for Tensile Properties of Polymer Matrix Composite Materials; ASTM: Englewood, CO, USA, American Society for Testing and Materials (ASTM). ASTM D 3410, Standard Test Method for Compressive Properties of Polymer Matrix Composite Materials with Unsupported Gage Section by Shear Loading; ASTM: Englewood, CO, USA, American Society for Testing and Materials (ASTM). ASTM D 5379, Standard Test Method for Shear Properties of Composite Materials by the VNotched Beam Method; ASTM: Englewood, CO, USA, American Society for Testing and Materials (ASTM). ASTM D 790, Standard Test Methods for Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials; ASTM: Englewood, CO, USA, International Standards Organization (ISO). ISO 155F, Fiberreinforced Plastic Composites Delamination of Flexural Properties; ISO: Geneva, Switzerland, Hoff, N.J.; Boley, B.A.; Coan, J.M. The development of a technique for testing stiff panels in edgewise compression. Proc. Soc. Exp. Stress Anal. 1948, 5, Park, J. Y. Finite Element analysis results of Shear buckling test of a Pultruded Composite ISection. Available online: (accessed on 27 August 2012) by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution license (
Journal of Composite Materials. Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios
Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios Journal: Manuscript ID: Draft Manuscript Type: Original Manuscript Date Submitted by the Author: n/a Complete List
More informationThe Local Web Buckling Strength of Coped Steel IBeam. ABSTRACT : When a beam flange is coped to allow clearance at the
The Local Web Buckling Strength of Coped Steel IBeam Michael C. H. Yam 1 Member, ASCE Angus C. C. Lam Associate Member, ASCE, V. P. IU and J. J. R. Cheng 3 Members, ASCE ABSTRACT : When a beam flange
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationDETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS. Abstract
DETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS Yixin Shao, Cynthia Giroux and Zeid Bdeir McGill University Montreal, Quebec, Canada Abstract The flexural rigidity, EI, plays an especially important
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationSize Effect of Clay Filler Particles on Mechanical Properties of Pultruded Polymer Composites Under Shear Loading
Minnesota State University, Mankato Cornerstone: A Collection of Scholarly and Creative Works for Minnesota State University, Mankato All Theses, Dissertations, and Other Capstone Projects Theses, Dissertations,
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationFinite Element Modelling with Plastic Hinges
01/02/2016 Marco Donà Finite Element Modelling with Plastic Hinges 1 Plastic hinge approach A plastic hinge represents a concentrated postyield behaviour in one or more degrees of freedom. Hinges only
More informationDEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8  PART 3 PROVISIONS
DEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8  PART 3 PROVISIONS Konstantinos CHRISTIDIS 1, Emmanouil VOUGIOUKAS 2 and Konstantinos TREZOS 3 ABSTRACT
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationCRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES
S. Kakay et al. Int. J. Comp. Meth. and Exp. Meas. Vol. 5 No. (017) 116 14 CRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES SAMDAR KAKAY DANIEL BÅRDSEN
More informationThe subject of this paper is the development of a design
The erformance and Design Checking of ChordAngle Legs in Joist Girders THEODORE V. GALAMBOS ABSTRACT The subject of this paper is the development of a design checking method for the capacity of the outstanding
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationFatigue failure mechanisms of thinwalled hybrid plate girders
Fatigue failure mechanisms of thinwalled hybrid plate girders Pavol Juhás1,* 1Institute of Technology and Business in České Budějovice, Department of Civil Engineering, Okružní 517/10, 37001 České Budějovice,
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationFatigue Resistance of Angle Shape Shear Connector used in SteelConcrete Composite Slab
Fatigue Resistance of Angle Shape Shear Connector used in SteelConcrete Composite Slab A dissertation submitted to the Graduate School of Engineering of Nagoya University in partial fulfillment of the
More informationSERVICEABILITY LIMIT STATE DESIGN
CHAPTER 11 SERVICEABILITY LIMIT STATE DESIGN Article 49. Cracking Limit State 49.1 General considerations In the case of verifications relating to Cracking Limit State, the effects of actions comprise
More informationEVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES
EVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES Koji YAMAGUCHI 1, Isao KIMPARA 1, and Kazuro KAGEYAMA 1 1 Department of Environmental &
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More informationEXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES
EXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES D. Kakogiannis 1, D. Van Hemelrijck 1, J. Wastiels 1, S. Palanivelu 2, W. Van Paepegem 2, K. De Wolf 3, J.
More informationAn Integrated Thermomechanical Method for Modeling Fiber Reinforced Polymer Composite Structures in Fire. Ziqing Yu¹ and Aixi Zhou²
An Integrated Thermomechanical Method for Modeling Fiber Reinforced Polymer Composite Structures in Fire Ziqing Yu¹ and Aixi Zhou² ¹Department of Engineering Technology, University of North Carolina at
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationMODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE
8th International DAAAM Baltic Conference INDUSTRIAL ENGINEERING 1921 April 2012, Tallinn, Estonia MODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE Pabut, O.; Allikas, G.; Herranen,
More informationA RATIONAL BUCKLING MODEL FOR THROUGH GIRDERS
A RATIONAL BUCKLING MODEL FOR THROUGH GIRDERS (Hasan Santoso) A RATIONAL BUCKLING MODEL FOR THROUGH GIRDERS Hasan Santoso Lecturer, Civil Engineering Department, Petra Christian University ABSTRACT Buckling
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationLap splice length and details of column longitudinal reinforcement at plastic hinge region
Lap length and details of column longitudinal reinforcement at plastic hinge region HongGun Park 1) and ChulGoo Kim 2) 1), 2 Department of Architecture and Architectural Engineering, Seoul National University,
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationENCE 455 Design of Steel Structures. III. Compression Members
ENCE 455 Design of Steel Structures III. Compression Members C. C. Fu, Ph.D., P.E. Civil and Environmental Engineering Department University of Maryland Compression Members Following subjects are covered:
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationBehavior of FRP BarsReinforced Concrete Slabs under Temperature and Sustained Load Effects
Polymers 14, 6, 873889; doi:1.339/polym63873 Article OPEN ACCESS polymers ISSN 73436 www.mdpi.com/journal/polymers Behavior of FRP BarsReinforced Concrete Slabs under Temperature and Sustained Load
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationELASTOPLASTIC STEEL BEAM BENDING ANALYSIS BY USING ABAQUS
11 ELASTOPLASTIC STEEL BEAM BENDING ANALYSIS BY USING ABAQUS Biswajit Jena * * Corresponding author: biswa.tech88@gmail.com Abstract: In recent years tremendous efforts have been made in development of
More informationFlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal Unbraced Lengths
Proceedings of the Annual Stability Conference Structural Stability Research Council San Antonio, Texas, March 2124, 2017 FlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal
More informationNONDESTRUCTIVE EVALUATION METHODS FOR COMPOSITE PILES
NONDESTRUCTIVE EVALUATION METHODS FOR COMPOSITE PILES John F. Davila Graduate Research Assistant 2006 URIUPRM SUMMER INTERNSHIP RESEARCH PROGRAM Kingstown, RI July 29 of 2006 PRESENTATION OUTLINE Introduction
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationAn Evaluation and Comparison of Models for Maximum Deflection of Stiffened Plates Using Finite Element Analysis
Marine Technology, Vol. 44, No. 4, October 2007, pp. 212 225 An Evaluation and Comparison of Models for Maximum Deflection of Stiffened Plates Using Finite Element Analysis Lior Banai 1 and Omri Pedatzur
More informationGeometrydependent MITC method for a 2node isobeam element
Structural Engineering and Mechanics, Vol. 9, No. (8) 33 Geometrydependent MITC method for a node isobeam element PhillSeung Lee Samsung Heavy Industries, Seocho, Seoul 37857, Korea HyuChun Noh
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationFormulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading
Formulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading Debaroti Ghosh & Mahbuba Begum Dept of Civil Engineering, Bangladesh University of Engineering
More informationThe stiffness tailoring of megawatt wind turbine
IOP Conference Series: Materials Science and Engineering OPEN ACCESS The stiffness tailoring of megawatt wind turbine To cite this article: Z M Li et al 2013 IOP Conf. Ser.: Mater. Sci. Eng. 52 052008
More informationINFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS
INFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS Paulo J. S. Cruz 1, Lúcio Lourenço 1, Hélder Quintela 2 and Manuel F. Santos 2 1 Department of Civil
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationModel tests and FEmodelling of dynamic soilstructure interaction
Shock and Vibration 19 (2012) 1061 1069 1061 DOI 10.3233/SAV20120712 IOS Press Model tests and FEmodelling of dynamic soilstructure interaction N. Kodama a, * and K. Komiya b a Waseda Institute for
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationStrainBased Design Model for FRPConfined Concrete Columns
SP230 57 StrainBased Design Model for FRPConfined Concrete Columns by N. Saenz and C.P. Pantelides Synopsis: A constitutive strainbased confinement model is developed herein for circular concrete columns
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationSeismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design
Seismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design Elmer E. Marx, Alaska Department of Transportation and Public Facilities Michael Keever, California Department
More informationEARTHQUAKE SIMULATION TESTS OF BRIDGE COLUMN MODELS DAMAGED DURING 1995 KOBE EARTHQUAKE
EARTHQUAKE SIMULATION TESTS OF BRIDGE COLUMN MODELS DAMAGED DURING 1995 KOBE EARTHQUAKE J. Sakai 1, S. Unjoh 2 and H. Ukon 3 1 Senior Researcher, Center for Advanced Engineering Structural Assessment and
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationProgram: Recent Trends
The SNL/MSU/DOE Fatigue Program: Recent Trends John Mandell Montana State University 2012 SNL Blade Workshop May 30  June 1, 2012 Outline Overview of MSU Fatigue Program on Wind Blade Materials: Testing
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationSUMMARY FOR COMPRESSION MEMBERS. Determine the factored design loads (AISC/LRFD Specification A4).
SUMMARY FOR COMPRESSION MEMBERS Columns with Pinned Supports Step 1: Step : Determine the factored design loads (AISC/LRFD Specification A4). From the column tables, determine the effective length KL using
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationStresses and Displacements in Functionally Graded Materials of SemiInfinite Extent Induced by Rectangular Loadings
Materials 2012, 5, 210226; doi:10.3390/ma5020210 Article OPEN ACCESS materials ISSN 19961944 www.mdpi.com/journal/materials Stresses and Displacements in Functionally Graded Materials of SemiInfinite
More informationBehavior and Modeling of Existing Reinforced Concrete Columns
Behavior and Modeling of Existing Reinforced Concrete Columns Kenneth J. Elwood University of British Columbia with contributions from Jose Pincheira, Univ of Wisconsin John Wallace, UCLA Questions? What
More informationDerivation of minimum steel ratio: based on service applied stresses
MATEC Web of Conferences, () DOI:./ matecconf/ Derivation of minimum steel ratio: based on service applied stresses Humam AL Sebai,*, Salah Al Toubat University of Sharjah, Sharjah city, UAE Abstract.
More informationMECHANICS OF MATERIALS
00 The McGrawHill Companies, Inc. All rights reserved. T Edition CHAPTER MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Teas Tech Universit
More informationPatch loading resistance of girders with corrugated webs
Patch loading resistance of girders with corrugated webs PhD Dissertation Balázs KÖVESDI Budapest University of Technology and Economics Supervisors: László DUNAI, DSc Professor Budapest University of
More informationAalto University School of Engineering
Aalto University School of Engineering Kul4.4 Ship Structural Design (P) ecture 6  Response of Webframes, Girders and Grillages Kul4.4 Ship Structures Response ecture 5: Tertiary Response: Bending
More informationBOOK OF COURSE WORKS ON STRENGTH OF MATERIALS FOR THE 2 ND YEAR STUDENTS OF THE UACEG
BOOK OF COURSE WORKS ON STRENGTH OF MATERIALS FOR THE ND YEAR STUDENTS OF THE UACEG Assoc.Prof. Dr. Svetlana LilkovaMarkova, Chief. Assist. Prof. Dimitar Lolov Sofia, 011 STRENGTH OF MATERIALS GENERAL
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationOptimum Design of Plate Girder
IOSR Journal of Mechanical and Civil Engineering (IOSRJMCE) eissn: 22781684,pISSN: 2320334X, Volume 13, Issue 6 Ver. III (Nov.  Dec. 2016), PP 2434 www.iosrjournals.org Optimum Design of Plate Girder
More informationHEALTH MONITORING OF PLATE STRUCTURE USING PIEZO ELECTRIC PATCHES AND CURVATURE MODE SHAPE
ISSN (Online) : 23198753 ISSN (Print) : 23476710 International Journal of Innovative Research in Science, Engineering and Technology An ISO 3297: 2007 Certified Organization, Volume 2, Special Issue
More informationA ratedependent HosfordCoulomb model for predicting ductile fracture at high strain rates
EPJ Web of Conferences 94, 01080 (2015) DOI: 10.1051/epjconf/20159401080 c Owned by the authors, published by EDP Sciences, 2015 A ratedependent HosfordCoulomb model for predicting ductile fracture at
More informationISO 178 INTERNATIONAL STANDARD. Plastics Determination of flexural properties. Plastiques Détermination des propriétés en flexion
INTERNATIONAL STANDARD ISO 178 Fifth edition 20101215 Plastics Determination of flexural properties Plastiques Détermination des propriétés en flexion Reference number ISO 178:2010(E) ISO 2010 PDF disclaimer
More informationARC 341 Structural Analysis II. Lecture 10: MM1.3 MM1.13
ARC241 Structural Analysis I Lecture 10: MM1.3 MM1.13 MM1.4) Analysis and Design MM1.5) Axial Loading; Normal Stress MM1.6) Shearing Stress MM1.7) Bearing Stress in Connections MM1.9) Method of Problem
More informationSTRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS
STRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS By Joseph F. Murphy 1 ABSTRACT: Four large glulam beams with notches on the tension side were tested for strength and stiffness. Using either bending
More informationVerification Examples. FEMDesign. version
FEMDesign 6.0 FEMDesign version. 06 FEMDesign 6.0 StruSoft AB Visit the StruSoft website for company and FEMDesign information at www.strusoft.com Copyright 06 by StruSoft, all rights reserved. Trademarks
More information